Carbohydrate Polymers 81 (2010) 372–376
Contents lists available at ScienceDirect
Carbohydrate Polymers journal homepage: www.elsevier.com/locate/carbpol
Synthesis and characterization of superparamagnetic chitosan–dextran sulfate hydrogels as nano carriers for colon-speciﬁc drug delivery Mohammad Reza Saboktakin a,b,∗ , Roya Tabatabaie a , Abel Maharramov b , Mohammad Ali Ramazanov b a b
Nanostructured Materials Synthesis Laboratory, International Research Institute of Arian Chemie Gostar, Tabriz, Iran Nanotechnology Research Center, Baku State University, Baku, Azerbaijan
a r t i c l e
i n f o
Article history: Received 8 February 2010 Received in revised form 12 February 2010 Accepted 19 February 2010 Available online 4 March 2010 Keywords: Chitosan Dextran sulfate Targeted drug delivery Hydrogels, Iron oxide nanoparticles
a b s t r a c t The purpose of this study was to examine chitosan (CS)–dextran sulfate (DS) nanoparticles coated iron oxide as drug carriers detectable using magnetic resonance imaging (MRI) technique. The 5aminosalicylic acid (5-ASA) was chosen as model drug molecule. CS–DS hydrogels were formulated by a complex coacervation process under mild conditions. The inﬂuence of process variables, including the two ionic polymers, on particle size, and hydrogel entrapment of 5-ASA was studied. The in vitro release of 5-ASA were also evaluated, and the integrity of 5-ASA in the release fraction was assessed using sodium dodecyl sulfate-polyacrylamide gel electrophoresis. The release of 5-ASA from hydrogel was based on the ion-exchange mechanism. The CS–DS hydrogel developed based on the modulation of ratio show promise as a system for controlled delivery of drug detectable using magnetic resonance imaging (MRI) technique. Crown Copyright © 2010 Published by Elsevier Ltd. All rights reserved.
1. Introduction Targeting of drugs speciﬁcally to the colon is advantageous in the treatment of diseases such as amoebiasis, Crohn’s disease, ulcerative colitis, and colorectal cancer. In addition, it has shown great potential in the oral delivery of therapeutic peptides and proteins, which are unstable in the upper part of the gastrointestinal (GI) tract. The colonic region is recognized as having less diversity and intensity of enzymatic activities than stomach and small intestine (Davis, 1990). Various strategies are available for targeting drug release selectively to the colon (Chourasia & Jain, 2003). The designing of prodrugs is based on the concept of preventing the release of drugs in the stomach and small intestine and drug release is triggered by the use of speciﬁc property at the target site such as altered pH or high activity of certain enzymes in comparison to nontarget tissues (Davaran, Hanaee, & Khosravi, 1999; Schacht et al., 1996). Since it is known that azo function can be reduced in the colon (Chung, Stevens, & Cerniglia, 1992), many novel polymers containing azo groups either in the polymeric backbone (Yamaoka, Makita, Sasatani, Kim, & Kimura, 2000) or in the cross-links (Shantha, Ravichandran, & Rao, 1995; Van den Mooter, Samyn, & Kinget, 1992) have been synthesized. To promote
∗ Corresponding author at: International Research Institute of Arian Chemie Gostar, Tabriz, Iran. Tel.: +994 984116694803; fax: +994 984116694803. E-mail address: [email protected]
further selective degradation in the vicinity of the colonic environment, delivery systems have been designed that contain both pH-sensitive acidic monomers and degradable azo aromatic crosslinks (Ghandehari, Kopeckova, & Kopecek, 1997; Kakoulides, Smart, & Tsibouklis, 1998). Chitosan is a functional linear polymer derived from chitin, the most abundant natural polysaccharide on the earth after cellulose, and it is not digested in the upper GI tract by human digestive enzymes (Furda, 1983; Ormrod, Holmes, & Miller, 1998). Chtosan is a copolymer consisting of 2-amino-2-deoxyd-glucose and 2-acetamido-2-deoxy-d-glucose units links with ␤-(1–4) bonds. It should be susceptible to glycosidic hydrolysis by microbial enzymes in the colon because it possesses glycosidic linkages similar to those of other enzymatically depolymerized polysaccharides. The polysaccharide, on reaching the colon, undergoes assimilation by microorganisms or degradation by enzymes or break down of the polymer back bone leading to a subsequent reduction in molecular weight and thereby loss of mechanical strength and is unable to hold the drug any longer (Yamamoto, Tozaki, Okada, & Fujita, 2000). Chitosan has drawn attention for its potential to achieve site-speciﬁc delivery to the colon. Chitosan, a natural linear polyamine with a high ratio of glucosamine to acetyl-glucosamine units, is a weak base and carriers a positive charge. Its solubility is pH-dependent, and it reacts readily with negatively charged surfaces and materials, including polymers and DNA. Ionic gelation, complex coacervation, emulsion crosslinking, and spray-drying are methods commonly used for the preparation of chitosan nanoparticles (Agnihotri, Mallikarjuna, &
0144-8617/$ – see front matter. Crown Copyright © 2010 Published by Elsevier Ltd. All rights reserved. doi:10.1016/j.carbpol.2010.02.034
M.R. Saboktakin et al. / Carbohydrate Polymers 81 (2010) 372–376
Aminabhavi, 2004). Among those methods, ionic gelation and complex coacervation are mild processes occurring in a pure aqueous environment and are ideal for maintaining the in-process stability of drugs. Ionic gelation and complex coacervation are very similar except that the former involves the gelation of chitosan using an electrolyte such as tripolyphosphate (TPP) (Calvo, RemunanLopez, Vila-Jato, & Alonso, 1997), whereas the latter employs an oppositely charged ionic polymer such as alginate (De & Robinson, 2003). A new type of chitosan (CS) hydrogel using dextran sulfate (DS) as a polyanionic polymer was developed to achieve complex coacervation for the incorporation and controlled release of an anti-angiogenesis hexapeptide (Chen, Mohanraj, & Parkin, 2003), this was the ﬁrst report describing the use of DS to formulate CSbased hydrogels. Although there have been investigations of how the properties of CS and formulation variables such as CS molecular weight (MW), concentrations of CS and 5-ASA, and formulation pH affect the formation and encapsulation capability of hydrogels (Ma, Yeoh, & Lim, 2002; Tiyaboonchai, Woiszwillo, Sims, & Middaugh, 2003), to our knowledge, no attempts have been made to study how the ratio of CS to the oppositely charged polymer inﬂuences the formulation and properties of hydrogel. In this study, 5aminosalicylic acid (5-ASA) was chosen as a model drug (Pan et al., 2002). 2. Materials and methods 2.1. Materials The polymer chitosan (medium MW 400,000 Da, 85% deacetylation) was purchased from Fluka/Sigma–Aldrich. Sodium salt of dextran sulfate (MW 12,750 Da), and 5-aminosalicylic acid were purchased from Sigma Chemical Co. All other solvents and materials were of analytical grade. Deionized water (Milli-Q water) was used in the preparation of buffers and standard solutions. All other chemicals and reagents used in this study were of analytical grade. 2.2. Methods 2.2.1. Preparation of superparamagnetic CS–DS hydrogel with 5-ASA Chitosan (CS) and dextran sulfate (DS) hydrogels were prepared using the method reported by Zhang et al., with slight modiﬁcations. Chitosan–dextran sulfate (at the charge ratio (N:P) of 1.12) and 35 mg FeCl3 ·6H2 O were solved in 4 mL H2 O and nitrogen was ﬂushed for 1.5 h. 14 mg FeCl2 ·4H2 O was added, followed by 100 L aqueous ammonia in two portions while the mixture was kept under nitrogen. The solution turned black and was heated to 80 ◦ C for 100 min. After the mixture cooled to room temperature, the ammonia was removed by ﬂushing the solution with nitrogen over 10 min. Then, the solid mixture was dissolved in 10 mL acetic acid (1%, w/v) and 5-aminosalicylic acid (5-ASA) (5–20 mg) was dissolved separately in dimethyl formamide (DMF). Then, the magnetic chitosan/dextran sulfate (2.5 mL) and the drug solution (7.5 mL) were mixed together to obtain 10 mL of chitosan/dextran sulfate drug solution. The chitosan/dextran sulfate drug solution was added dropwise (using a disposable syringe with a 22-gauge needle) into 40 mL of sodium-saturated Tris–HCl buffer solution containing glutaraldehyde-saturated toluene (GST) in different concentrations (1–3 mL) under magnetic stirring (∼200 rpm) at room temperature. The hydrogel suspension was formed spontaneously. The mixture was stirred for a further 15 min. The hydrogel was separated after 1 h of curing time and subsequently decanted, washed twice with 3 mL of 0.05 M Tris–HCl buffer, and the hydrogel was dried in vacuum oven at 40 ◦ C.
2.2.2. Shape and surface morphology Surface and shape characteristics of chitosan–dextran sulfate hydrogels were evaluated by means of a scanning electron microscope (FEI-Qunta-200 SEM, FEI Company, Hillsboro, OR). The samples for SEM were prepared by lightly sprinkling the hydrogel on a bouble adhesive tape, which stuck to an aluminum stub. The stubs were than coated with gold to a thickness of ∼300 Å using a sputter coater and viewed under the scanning electron microscope. 2.2.3. Particle size After drying at 37 ◦ C for 48 h, the mean diameter of the dried hydrogel was determined by a sieving method using USP standard sieves. Observations are recorded. 2.2.4. Drug content and encapsulation efﬁciency Encapsulation efﬁciency (EE) is the amount of added drug (%) that is encapsulated in the formulation of the hydrogel. The EE of drug from hydrogel can be calculated in terms of the ratio of drug in the ﬁnal formulation to the amount of added drug. An accurately weighed amount (100 mg) of the formulation of hydrogel was dispersed in 100 mL of Tris–HCl buffer. The sample was ultrasonicated for three consecutive periods of 5 min each, with a resting period of 5 min each. It was left to centrifuged at 3000 rpm for 15 min. The concentration of 5-aminosalicylic acid (5-ASA) in the decanted Tris–HCl buffer and two washing solutions was determined by measuring the absorbance at 235 nm using a GBS Cintra 10-UV–visible spectrophotometer (Shimadzu, Japan). The determinations were made in triplicate, and results were averaged (Table 1). 2.2.5. Equilibrium swelling studies Chitosan–dextran sulfate hydrogels (100 mg) were placed in phosphate buffered saline (PBS) (pH 7.4) and allowed to swell upto a constant weight. The hydrogels were removed, blotted with ﬁlter paper, and changes in weight were measured and recorded in Table 1. The degree of swelling (˛) was then calculated from the formula: Wg − Wo Wo where, Wo is the initial weight of hydrogel and Wg is the weight of hydrogel at equilibrium swelling in the medium. 2.2.6. In vitro drug release study of 5-ASA-loaded hydrogel In vitro drug release studies were performed according to extraction technique using USP dissolution test apparatus. The dissolution studies were performed in 900 mL of dissolution medium, which was stirred at 100 rpm at 37 ± 0.1 ◦ C. The scheme of using the simulated ﬂuids at different pH was as follows: • First hour: simulated gastric ﬂuid of pH 1.2 • Second to third hour: mixture of simulated gastric and intestinal ﬂuid of pH 4.5 • Fourth to Fifth hour: simulated intestinal ﬂuid of pH 7.4 • Sixth to eighth hour: simulated colonic ﬂuid of pH 7.0 In vitro drug release studies were performed as per the scheme in different simulated ﬂuids. Simulation of GI transit conditions was achieved by using different dissolution media. Simulated gastric ﬂuid (SGF) pH 1.2 consisted of NaCl (0.2 g), HCl (7 mL), and pesin (3.2 g); pH was adjusted to 1.2 ± 0.5. Simulated intestinal ﬂuid (SIF) pH 7.4 consisted of KH2 PO4 (6.8 g), 0.2 N NaOH (190 mL), and pancreatin (10.0 g); pH was adjusted to 7.4 ± 0.1. SIF pH 4.5 was prepared by mixing SGF pH 1.2 and SIF pH 7.4 in a ratio of 36:61. The experiment was performed with a continuous supply
M.R. Saboktakin et al. / Carbohydrate Polymers 81 (2010) 372–376
Table 1 Compositions and characteristics of different chitosan–dextran sulfate hydrogel. Variables
Degree of swelling
0 5 10 15 20
1.36 1.24 1.00 0.95 0.68
± ± ± ± ±
0.05 0.20 0.01 0.09 0.12
1.20 1.68 1.70 1.92 1.20
± ± ± ± ±
0.08 0.08 0.06 0.04 0.10
– 74.8 ± 75.2 ± 80.1 ± 85.6 ±
2.34 1.98 2.54 1.63
CS–DS hydrogel (%w/w)
1 2 3 4
1.10 1.20 1.32 1.50
± ± ± ±
1.00 1.21 1.35 1.40
1.38 1.75 1.90 1.87
± ± ± ±
0.11 0.09 0.05 0.02
80.8 82.3 86.7 88.7
± ± ± ±
3.24 1.25 2.47 2.35
10 min 20 min 40 min
0.50 ± 0.52 0.53 ± 0.14 0.85 ± 0.05
1.90 ± 0.12 1.87 ± 0.21 1.70 ± 0.32
70.3 ± 1.47 86.4 ± 1.98 76.7 ± 2.45
Drying (◦ C)
0.86 ± 0.50 0.71 ± 0.72
1.32 ± 0.12 1.00 ± 0.64
69.8 ± 4.35 65.4 ± 3.98
of carbon dioxide into dissolution media. Aliquots of samples were withdrawn periodically and replaced with an equal amount of fresh dissolution media bubbled with carbon dioxide. The volume was made upto 10 mL and centrifuged. The supernatant was ﬁltered through Whatman ﬁlter paper (Dawsonville, GA), and drug content was determined spectrophotometrically at 235 nm (UV 1601, Shimadzu, Japan).
Average particle size (mm)
Encapsulation efﬁciency (%)
2.2.8. Conductivity measurement Conductivity of hydrogel dispersion, 0.1% CS, 0.1%DS with iron oxide nanoparticles in the deionized water was determined using a conductivity meter (Systronics 307) with a conductivity range from 0.1 to 200 m at room temperature. All samples were prepared in deionized water. 3. Results and discussion
2.2.7. Statistical analysis Experimental data have been represented as the mean with standard deviation (SD) of different independent determinations. The signiﬁcance of differences was evaluated by analysis of variance (ANOVA). Differences were considered statistically signiﬁcant at P < 0.005.
3.1. Hydrogel characteristics These hydrogels had good spherical geometry. It is obvious that the surface of the hydrogel shrank and a densely cross-linked gel structure was formed. This may explain the greater retardation
Fig. 1. Morphology of chitosan–dextran sulfate (CS–DS) hydrogel by emission scanning electron microscopy ﬁeld.
M.R. Saboktakin et al. / Carbohydrate Polymers 81 (2010) 372–376
of drug release from matrices of higher cross linker content. The average drug entrapment was found to be 81.21 ± 1.86% in the hydrogel. 3.2. Drug content and encapsulation efﬁciency Results of drug content and EE demonstrated that drug content increased from 10.23 ± 0.50 mg/100 mg to 26.24 ± 0.43 mg/100 mg of hydrogel with increasing the amount of drug from 5 to 20% (w/w). No signiﬁcation increase in drug content was observed on further increasing the amount of drug, i.e., above 15% (w/w), which could be due to the limited solubility of the drug in DMF and that is endorsed from the presence of drug particles on the surface of the hydrogel prepared with 20% of drug concentration. The percent EE was increased upto 86.32 ± 0.20% with increasing polymer concentrations to 4%. Concentration of the cross-linking agent exhibited no signiﬁcant effect on percent EE.
Fig. 3. The in vitro release proﬁle of 5-aminosalicylic acid from chitosan–dextran sulfate hydrogel in various simulated gastrointestinal ﬂuids (n = 3).
3.3. Morphology of superparamagnetic CS–DS hydrogel FESEM images of superparamagnetic CS–DS hydrogel (Fig. 1) show that hydrogel have a solid and near consistent structure. Furthermore, the incorporation of 5-ASA into the hydrogel produced a smooth surface and compact structure. The particle size observed in FESEM is smaller than that measured by the Zetasizer. This is because dried hydrogel was used in FESEM, whereas particles in the liquid dispersion was analyzed by the Zetasizer. CS–DS hydrogel are hydrophilic and would be expected to swell in water, thus producing a large hydrodynamic size when measured by the Zetasizer (Fig. 2). 3.4. Incorporation of 5-ASA into CS–DS hydrogel 5-aminosalicylic acid (5-ASA)-loaded hydrogel was obtained spontaneously upon the mixing of the DS aqueous solution (0.1%, w/v) with the CS solution (0.1%, w/v) under magnetic stirring, with 5-ASA dissolved in CS–DS solution. The incorporation of 5-ASA into the CS–DS hydrogel resulted in a sharp increase in the particle size of the nanoparticle dispersion. The signiﬁcant increases in particle size give a good induction of the incorporation of 5-ASA into CS–DS hydrogel. A study was undertaken to investigate the effect of the order of 5-ASA mixing with CS and DS. The data obtained show that the order of 5-ASA mixing had no effect on the size, entrapment efﬁciency, and yield of 5-ASA-loaded hydrogel.
Fig. 2. Inﬂuence of the chitosan:dextran sulfate ratio on the particle size.
3.5. In vitro release studies The effect of drug concentration, chitosan–dextran sulfate concentration, GST concentration, and cross-linking time on in vitro drug release was also observed. In vitro drug release after 5 h was 86.3 ± 4.0% in the case of hydrogel having 15% drug, while it was 88.2 ± 3.1% for hydrogel with 20% drug. The effect of chitosan–dextran sulfate on the release of drug was found to be meager. It is also observed that the amount of drug released from hydrogel decreased on increasing cross-linking time. These properties are probably explained by the promotion of cross-links between chitosan–dextran sulfate chains and GST. Freeze-drying of the samples resulted in larger and more porous hydrogel compared with air-dried hydrogel. Freeze-drying had the advantage of avoiding drug extraction by immediately freezing and removing the water present within the hydrogel and a burst effect during the dissolution study (Fig. 3). Conventional dissolution testing is less likely to accurately predict in vivo performance of colon delivery systems triggered by bacteria residing in the colon (because aspects of the colon’s environment, i.e., scarcity of ﬂuid, reduced motility, and presence of microﬂora, cannot be simulated in conventional dissolution methods). Hence, release studies were performed in an alternate release medium. The release proﬁles of 5-ASA-loaded hydrogel was evaluated in water and a phosphate buffer, which was either in a different ionic strength or with saline, to study the
Fig. 4. In vitro drug release from chitosan–dextran sulfate hydrogel in SCF (pH 7.0) in presence 5-ASA.
M.R. Saboktakin et al. / Carbohydrate Polymers 81 (2010) 372–376
Table 2 Conductivity of dispersion of hydrogel in the different pH. Weight ratio of CS:DS
Charge ratio (N:P) of the hydrogel
pH of hydrogel
Conductivity of dispersion (in m)
Size (in nm)
5:4.5 5:5 5:8.5
1.01 1.12 1.90
4.0 3.9 4.1
3.72 3.70 3.78
1892 350 240
underprinning mechanisms for drug release. The greatest release for 5-ASA–loaded hydrogel occurred in the release media of a high ionic strength. In contrast, a signiﬁcantly small portion of 5-ASA was released in water over the release study period. The burst release was observed with hydrogel, and it may have arisen from the desorption of loosely attached 5-ASA from the surface of the matrix polymers (Fig. 4). 3.6. Hydrogel conductivity studies The opposite charges of CS–DS hydrogel were responsible for the formation of nanoparticles. The charge ration between the negatively charged sulfate groups (N) in DS and the positively charged amine groups (P) in CS was determined. Under the experimental conditions (pH 3–4), DS carries ∼74 sulfate groups per mole, equivalent to 5.78 × 10−3 negatively charged groups per gram of DS; CS has ∼2073 amino groups per gram of CS. Table 2 shows conductivity of dispersion of hydrogel. 4. Conclusion Results of release studies indicate that superparamagnetic chitosan–dextran sulfate hydrogel offer a high degree of protection from premature drug release in simulated upper conditions. These hydrogels deliver most of the drug load in the colon, an environment rich in bacterial enzymes that degrade the chitosan–dextran sulfate and allow drug release to occur at the desired site. Thus, spherical superparamagnetic hydrogel is a potential system for colon delivery of 5-ASA. Also, this hydrogel can be detect by magnetic resonance imagining (MRI) technique. References Agnihotri, S. A., Mallikarjuna, N. N., & Aminabhavi, T. M. (2004). Recent advances on chitosan-based micro- and nanoparticles in drug delivery. Journal of Controlled Release, 100, 5–28. Calvo, P., Remunan-Lopez, C., Vila-Jato, J. L., & Alonso, M. J. (1997). Novel hydrophilic chitosan-polyethylene oxide nanoparticles as protein carriers. Journal of Applied Polymer Science, 63, 125–132.
Chen, Y., Mohanraj, V., & Parkin, J. (2003). Chitosan–dextransulfate nanoparticles for delivery of an anti-angiogenesis peptide. International Journal of Peptide Research and Therapeutics, 10, 621–629. Chourasia, M. K., & Jain, S. K. (2003). Pharmaceutical approaches to colon targeted drug delivery systems. Journal of Pharmaceutical Sciences, 6, 33–66. Chung, K. T., Stevens, S. E., & Cerniglia, C. E. (1992). The reduction of azo dyes by the intestinal microﬂora. Critical Reviews of Microbiology, 18, 175–190. Davaran, S., Hanaee, J., & Khosravi, A. (1999). Release of 5-aminosalicylic acid from acrylic type polymeric prodrugs designed for colon-speciﬁc drug delivery. Journal of Controlled Release, 58, 279–287. Davis, S. S. (1990). Assessment of gastrointestinal transit and drug absorption. In L. F. Prescott, & W. S. Nimmo (Eds.), Novel drug delivery and its therapeutic application (pp. 89–101). Chichester, UK: Wiley. De, S., & Robinson, D. (2003). Polymer relationships during preparation of chitosanalginate and poly-l-lysine-alginate nanospheres. Journal of Controlled Release, 89, 101–112. Furda, I. (1983). Aminopolysaccharides—their potential as dietary ﬁber. In I. Furda (Ed.), Unconventional sources of dietary ﬁber, physiological and in vitro functional properties (pp. 105–122). Washington, DC: American Chemical Society. Ghandehari, H., Kopeckova, P., & Kopecek, J. (1997). In vitro degradation of pH sensitive hydrogels containing aromatic azo bonds. Biomaterials, 18, 861–872. Kakoulides, E. P., Smart, J. D., & Tsibouklis, J. (1998). Azo crosslinked poly(acrylic acid) for colonic delivery and adhesion speciﬁcity synthesis and characterization. Journal of Controlled Release, 52, 291–300. Ma, Z., Yeoh, H. H., & Lim, L. Y. (2002). Formulation pH modulates the interaction of insulin with chitosan nanoparticles. Journal of Pharmaceutical Sciences, 91, 1396–1404. Ormrod, D. J., Holmes, C. C., & Miller, T. E. (1998). Dietary Chitosan inhibits hypercholesterolaemia and atherogenesis in the apolipoprotein E-deﬁcient mouse model of atherosclerosis. Atherosclerosis, 138, 329–334. Pan, Y., Li, j., & Zhao, H. (2002). Bioadhesive polysaccharide in protein delivery system: Chitosan nanoparticles improve the intestinal absorption of insulin in vivo. International Journal of Pharmaceutics, 24, 139–147. Schacht, E., Gevaert, A., & Kenawy, E. R. (1996). Polymers for colon speciﬁc drug delivery. Journal of Controlled Release, 58, 327–338. Shantha, K. L., Ravichandran, P., & Rao, K. P. (1995). Azo polymeric hydrogels for colon targeted drug delivery. Biomaterials, 16, 1313–1318. Tiyaboonchai, W., Woiszwillo, J., Sims, R. C., & Middaugh, C. R. (2003). Insulin containing polyethylenimine-dextran sulfate nanoparticles. Journal of Pharmaceutical Sciences, 255, 139–151. Van den Mooter, G., Samyn, C., & Kinget, R. (1992). Azo polymers for colon-speciﬁc drug delivery. International Journal of Pharmaceutics, 87, 37–46. Yamamoto, A., Tozaki, H., Okada, N., & Fujita, T. (2000). Colon speciﬁc delivery of peptide drugs and anti-inﬂammatory drugs using chitosan capsules. STP Pharma Science, 10, 23–43. Yamaoka, T., Makita, Y., Sasatani, H., Kim, S. I., & Kimura, Y. (2000). Linear type azocontaining polyurethane as drug-coating material for colon-speciﬁc delivery: Its properties degradation behavior and utilization for drug formulation. Journal of Controlled Release, 66, 187–197.